Concrete maturity is an index value that represents the progression of concrete curing. It is based on an equation that takes into account concrete temperature, time, and strength gain. Concrete maturity is an accurate way to determine real-time strength values of curing concrete.

Early, rapid, and accurate in-situ estimation of the compressive strength of concrete is one of the major challenges for the concrete industry. A practical solution for such challenges can prevent millions of dollars of extra annual spending for the construction industry and owners of civil structures.

The maturity method is a convenient approach to predict the early age strength gain of concrete, using the principle that the concrete strength is directly related to the hydration temperature history of cementitious paste. The maturity concept for estimating the strength gain of concrete is described in ASTM C1074, Standard Practice for Estimating Concrete Strength by the Maturity Method. This method can potentially address many immediate challenges facing the concrete industry such as predicting appropriate time for formwork stripping and post-tensioning, especially at low temperatures while the strength development of concrete is hindered; and optimizing concrete mix design and concrete curing conditions (e.g. concrete heating at low temperatures or surface protection in hot-dry weathers).

Lack of an accurate estimation of strength at early ages of construction is twofold: contractors either wait too long for next action (e.g. stripping formwork) which is costly due to delays in completing the project, or they act prematurely which could cause the concrete structure to crack - that would lead to future durability and performance issues - or even structural collapse.

In most construction sites, field-cured concrete samples are tested to strength at various ages during the first week since concrete is poured, in order to make a decision on formwork removal. Usually, if the concrete reaches 75% of its designed strength, the structural engineers allow for the striping of forms. The problem, however, is that only one specimen is crushed for strength estimation. This is not necessarily accurate.

In addition, the construction crew is usually on the job site while they are waiting to hear about the compressive strength result from the lab. This adds to the cost of construction and its uncertainty decreases the efficiency of the construction. Although alternative methods such as concrete maturity exist, there is a traditional resistance to utilizing them for most concrete projects. Except for specific projects, the concrete industry shows interest in the commonly used compressive strength test. This is mainly due to the upfront cost of concrete mixture calibration for maturity curves, and lack of expertise for the installation of concrete temperature sensors, data collection and analysis.

Such approaches to compressive strength evaluation may cause concrete contractors to make conservative decisions, face more complicated technical problem (e.g. delay in formwork stripping, and unnecessary long-term curing and surface protection), and spend more financial resources.

As a non-destructive testing, the maturity method may be a reasonable candidate to fill this gap. In comparison to most on-site non-destructive technologies (e.g. Schmidt Hammer or Ultrasonic Pulse Velocity), the privilege that the maturity method stands on is that, the procedure for estimating the compressive strength would be objective and qualitative once the maturity curve is developed and adopted.

This technical article describes how the maturity curve is developed, and how it is applied for on-site estimation of the compressive strength of concrete.

Maturity method is a relatively simple approach for estimating the in-place compressive strength of concrete, specifically at early ages less than 14 days. Once the maturity curve is developed in the laboratory for a specific project, it can be used for on-site estimation of compressive strength of concrete in real-time.

The maturity method is governed by the fundamental assumption that a given concrete mix design poured during course of a specific project has the same compressive strength when it has the same “maturity index”. It means that a given concrete mix design, for example, may reach the same compressive strength after 7 days of curing at 10 °C when it is cured at 25 °C for 3 days.

The maturity method based on the ASTM C1074 is the most commonly used method to estimate the in-situ strength of concrete. ASTM C1074 provides two maturity functions: 1) Nurse-Saul function; and 2) Arrhenius function. Based on the Nurse-Saul method, there is a linear relationship between the maturity and the temperature in real time. The underlying assumption is that the strength development in concrete is a linear function of hydration temperature. Equation 1 shows the relationship between maturity and hydration temperature history.

Where: M(t) is the maturity index at age t; T_{a} is the average temperature during time interval ∆t; T_{0} is the datum temperature. ASTM C1074 provides a standard procedure to find the datum temperature for a specific mix design. However, most of previous studies suggest a practical estimation of the datum temperature that is between 0 °C and -10 °C. Indeed, this is the temperature at which the hydration of cementitious paste stops; hence the strength development of concrete ceases. Unpublished results by Giatec Scientific Inc. show that this temperature resides within an interval between 0 °C and -5 °C dependent on the concrete mix design.

The second approach is the Arrhenius function that assumes there is an exponential relationship between the compressive strength and hydration temperature. The maturity index is defined in form of an equivalent age at a reference temperature. It means the actual age should be normalized to the reference temperature in order to estimate the compressive strength. This function needs a value of activation energy that can be determined as the procedure detailed in ASTM C1074.

Despite the fact that the Arrhenius function is scientifically more accurate, the Nurse-Saul function is more commonly used by concrete industry because of the following reasons:

- The accuracy of the Nurse-Saul function is adequate for most field applications;
- The Nurse-Saul function is relatively simpler compared with the Arrhenius function.

As detailed in ASTM C1074, there is a step-by-step guide for developing the maturity curve, and for estimating the compressive strength. These steps are described as follows.

The maturity-strength curve represents the relationship between maturity index and compressive strength for a specific concrete mix design, adopted in the laboratory. To do so, adequate concrete cylindrical specimens should be casted, and then stored in the semi-adiabatic condition for curing. Certain number of concrete cylinders (i.e. at least two concrete specimens) should be equipped by embedded temperature sensors for recording the hydration temperature history. The compressive strength of concrete is measured at ages of 1, 3, 7, 14 and 28 days.

- In-place concrete is not representative of the concrete used to develop the calibration in the lab. This can be because of changes in materials, water to cement ration, air content, batching method, etc;
- In-place concrete is not properly placed, consolidated, cured, etc;
- Very high early-age temperatures can lead to inaccurate estimation of strength at later ages;
- Using a datum temperature (for the Nurse-Saul function) that is not representative of the concrete mixture can result in incorrect estimation of strength.